Fracture Modes• Simple fracture is the separation of a body into 2 or more pieces in response to an applied stress that is static (constant) and at temperatures that are low relative to the Tm of the material.• Classification is based on the ability of a material to experience plastic deformation.• Ductile fracture – Accompanied by significant plastic deformation• Brittle fracture – Little or no plastic deformation – Sudden, catastrophic 3
Fracture Mechanism Imposed stress Crack Formation Propagation• Ductile failure has extensive plastic deformation in the vicinity of the advancing crack. The process proceeds relatively slow (stable). The crack resists any further extension unless there is an increase in the applied stress.• In brittle failure, cracks may spread very rapidly, with little deformation. These cracks are more unstable and crack propagation will continue without an increase in the applied stress. 4
Crack PropagationCracks propagate due to sharpness of crack tip• A plastic material deforms at the tip, “blunting” the crack. deformed region brittle plasticEnergy balance on the crack• Elastic strain energy- • energy stored in material as it is elastically deformed • this energy is released when the crack propagates • creation of new surfaces requires energy 5
Ductile vs Brittle Failure Fracture Very Moderately Brittle behavior: Ductile Ductile %AR or %EL Large Moderate Small• Ductile fracture is Ductile: Brittle: usually more desirable Warning before No than brittle fracture. fracture warning 6
Moderately Ductile Failure• Evolution to failure: void Coalescence Crack fracture necking nucleation of cavities propagation• Resulting 50 mm 50 mm fracture surfaces (steel) 100 mmparticles From V.J. Colangelo and F.A. Heiser, Analysis of Fracture surface of tire cord wire loaded in tension. Metallurgical Failures (2nd ed.), Fig. 11.28, p. 294, John Courtesy of F. Roehrig, CC Technologies, Dublin, OH.serve as void Wiley and Sons, Inc., 1987. (Orig. source: P. Thornton, J. Used with permission. Mater. Sci., Vol. 6, 1971, pp. 347-56.)nucleationsites. 7
Example: Pipe Failures • Ductile failure: -- one piece -- large deformation • Brittle failure: -- many pieces -- small deformationsFigures from V.J. Colangelo and F.A. Heiser, Analysis ofMetallurgical Failures (2nd ed.), Fig. 4.1(a) and (b), p. 66 JohnWiley and Sons, Inc., 1987. Used with permission. 8
Ductile vs. Brittle Failurecup-and-cone fracture brittle fracture 9
Ductile Failure(a) SEM image showing spherical dimples resultingfrom a uniaxial tensile load. (b) SEM image ofparabolic dimples from shear loading. 10
Brittle FractureArrows indicate point at failure originationDistinctive pattern on the fracture surface: V-shaped “chevron” markings point to the failureorigin. 11
Transgranular Fracture• Cleavage - in most brittle crystalline materials, crack propagation that results from the repeated breaking of atomic bonds along specific planes.• This leads to transgranular fracture where the crack splits (cleaves) through the grains. 12
Intergranular Fracture• Intergranular failure is typically due to elemental depletion (chromium) at the grain boundaries or some type of weakening of the grain boundary due to chemical attack, oxidation, embrittlement. 13
Stress Concentration• The measured fracture strengths for most brittle materials are significantly lower than those predicted by theoretical calculations based on atomic bond energies.• This discrepancy is explained by the presence of very small, microscopic flaws or cracks that are inherent to the material.• The flaws act as stress concentrators or stress raisers, amplifying the stress at a given point.• This localized stress diminishes with distance away from the crack tip.
Fracture Toughness• Fracture toughness measures a material’s resistance to brittle fracture when a crack is present.• It is an indication of the amount of stress required to propagate a preexisting flaw.• Flaws may appear as cracks, voids, metallurgical inclusions, weld defects, design discontinuities, or some combination thereof.• It is common practice to assume that flaws are present and use the linear elastic fracture mechanics (LEFM) approach to design critical components.• This approach uses the flaw size and features, component geometry, loading conditions and the fracture toughness to evaluate the ability of a component containing a flaw to resist fracture.
Ductile vs Brittle• The effect of a stress raiser is more significant in brittle than in ductile materials.• For a ductile material, plastic deformation results when the maximum stress exceeds the yield strength.• This leads to a more uniform distribution of stress in the vicinity of the stress raiser; the maximum stress concentration factor will be less than the theoretical value.• In brittle materials, there is no redistribution or yielding.
stress-intensity factor (K)• The stress-intensity factor (K) is used to determine the fracture toughness of most materials.• A Roman numeral subscript indicates the mode of fracture and the three modes of fracture are illustrated in the image to the right.• Mode I fracture is the condition where the crack plane is normal to the direction of largest tensile loading. This is the most commonly encountered mode.• The stress intensity factor is a function of loading, crack size, and structural geometry. The stress intensity factor may be represented by the following equation:KI is the fracture toughness inσ is the applied stress in MPa or psia is the crack length in meters or inchesβ is a crack length and component geometry factor that is different for each specimen, dimensionless.
Critical Stress• All brittle materials contain a population of small cracks and flaws that have a variety of sizes, geometries and orientations.• When the magnitude of a tensile stress at the tip of one of these flaws exceeds the value of this critical stress, a crack forms and then propagates, leading to failure.• Condition for crack propagation: K ≥ Kc Stress Intensity Factor: Fracture Toughness: --Depends on load & geometry. --Depends on the material, temperature, environment & rate of loading. Fracture toughness - good diagrams http://www.ndt-ed.org/EducationResources/CommunityCollege/Materials/Mechanical/FractureToughness.htm 20
Compact tension (CT) specimen single edge notch bend (SENB or three-point bend)
Flaws are Stress Concentrators If the crack is similar to an elliptical hole through plate, and is oriented perpendicular to applied stress, the maximum stress σm= 1/ 2 a σ =2σ =Ktσ m o ρ t oρt where ρt = radius of curvature σo = applied stress σm = stress at crack tip a = length of surface crack or ½ length of internal crack σm / σo = Kt the stress concentration factor 22
DESIGN AGAINST CRACK GROWTH• Crack growth condition: K ≥ Kc Yσ πa• Largest, most stressed cracks grow first. --Result 1: Max flaw size --Result 2: Design stress dictates design stress. dictates max. flaw size. Kc 1 K 2 σdesign < a max < c Y πa max π Yσdesign amax σ fracture fracture no no fracture amax fracture σ
Design Example: Aircraft Wing• Material has Kc = 26 MPa-m0.5• Two designs to consider... Design A Design B -- largest flaw is 9 mm -- use same material -- failure stress = 112 MPa -- largest flaw is 4 mm Kc -- failure stress = ?• Use... σc = Y πamax• Key point: Y and Kc are the same in both designs. Y is a dimensionless parameter; see Callister page 298. -- Result: 112 MPa 9 mm 4 mm ( σc ) amax A = σc amax B ( ) Answer: (σc )B = 168 MPa• Reducing flaw size pays off. 24
Sensors made to mesh with plane• Structural engineers have long imagined the day when materials used in an aircraft, a wind turbine blade or a bridge could sense if they had been strained to the point of damage, reducing their load-carrying capacity, and report that information in real time before the structures safety is compromised.• For many years, such a scenario was more the stuff of science fiction than fact, but today, structural health monitoring (SHM) systems that can perform these tasks are closer to reality.• Scientists have created a fiber mesh embedded with sensors designed to monitor an airplane’s structural integrity and outside temperature.• When wrapped around an aircraft, the sensors could help prevent microscopic cracks from developing into catastrophic failures.• Made from a plastic polymer, the mesh is designed so it doesn’t add significant weight or drag to an aircraft.• The technology also could be used in autos, packaging and medical devices.
Structural health monitoring (SHM) A piezoelectric-based sensor system systems can be arrayed in similar from Acellent Technologies, called fashion to the human nervous system, SMART Layer, identifies damage with with sensors concentrated in key areas small ceramic actuators where loads are highest. An FAA-sponsored study on curvedA comparative vacuum-monitoring (CVM) honeycomb-cored panels showed thatsensor, is a thin, self-adhesive rubber patch acoustic emission (AE) monitoring is athat detects cracks in the underlying material. reliable method for locating damage initiationThe rubber is laser-etched with rows of tiny, sites and for tracking crack progression.interconnected channels or galleries, to which Source: Physical Acoustics Corpan air pressure is applied. Any propagatingcrack under the sensor breaches the galleriesand the resulting change in pressure ismonitored. http://www.compositesworld.com/articles/structural-health-monitoring-composites-get-smart http://www.photonics.com/Article.aspx?AID=30528
Brittle Fracture of Ceramics• Most ceramics (at room temperature) fracture before any plastic deformation can occur.• Typical crack configurations for 4 common loading methods. 28
Brittle Fracture of Ceramics• Surface of a 6-mm diameter fused silica rod.• Characteristic fracture behavior in ceramics – Origin point – Initial region (mirror) is flat and smooth – After reaches critical velocity crack branches • mist • hackle 29
Fracture of PolymersThe fracture strengths of polymers are low relative to ceramics andmetals.The fracture mode in thermosetting polymers (heavily crosslinkednetworks) is typically brittle.For thermoplastic polymers, both ductile and brittle modes are possible.Reduced temperature, increased strain rate, sharp notches, increasedspecimen thickness are some factors that can influence a brittle fracture.One phenomenon that occurs in thermoplastics is crazing, very localizedplastic deformation and formation of microvoids and fibrillar bridges aligned chains fibrillar bridges microvoids crack 30
Impact Testing• Impact loading: (Charpy) -- severe testing case -- makes material more brittle -- decreases toughness final height initial height 31
Ductile to Brittle Transition Temperature (DBTT)• Pre-WWII: The Titanic • WWII: Liberty ships Disastrous consequences for a welded transport ship, suddenly split across the entire girth of the ship (40˚F). The vessels were constructed from steel alloys that exhibit a DBTT ≈ room tempReprinted w/ permission from R.W. Hertzberg, "Deformation and Fracture Mechanics of Engineering Materials", (4th ed.) Fig. 7.1(a), p. 262, John Wiley and Sons,Inc., 1996. (Orig. source: Dr. Robert D. Ballard, The Discovery of the Titanic.) 32
Charpy Impact Energy (A) and Shear Fracture % (B) Correlated with Temperature 33
Steel Charpy SamplesFracture surfaces after impact showingthe variation in ductility with testingtemperature (˚C). 34
Temperature • Increasing temperature... -- increases %EL and Kc • Ductile-to-Brittle Transition Temperature (DBTT)... FCC metals (e.g., Cu, Ni)Impact Energy BCC metals (e.g., iron at T < 914°C) polymers Brittle More Ductile High strength materials (σ y > E/150) Temperature Ductile-to-brittle transition temperature 35
Fatigue Fatigue testing apparatus for rotating bending testFatigue is a form of failure that occurs in structures subjectedto dynamic stresses over an extended period.Under these conditions it is possible to fail at stress levelsconsiderably lower than tensile or yield strength for a staticload.Single largest cause of failure in metals; also affectspolymers and ceramics.Common failure in bridges, aircraft and machinecomponents. 36
Cyclic Stress - Fatigue• Variation of stress with time that accounts for fatigue failures.• The stress may be axial (tension- compression), flexural (bending) or torsional (twisting) in nature.• There are 3 fluctuating stress- time modes seen in the figure: (a) reversed stress cycle - symmetrical amplitude about a mean zero stress level; (b) repeated stress cycle - asymmetrical maxima and minima relative to the zero stress level; (c) variable (random) stress level 37
Fatigue• Fracture surface with crack initiation at top. Surface shows predominantly dull fibrous texture where rapid failure occurred after crack achieved critical size.• Fatigue failure 1. Crack initiation 2. Crack propagation 3. Final failure 38
• Striations are closetogether indicatinglow stress, many cycles.• Widely spaced striations • Fatigue failure is brittle in nature, even in normally ductile materials; there is verymean high stress few little plastic deformation associated withcycles. the failure. • The image shows fatigue striations 39 (microscopic).
• Federal investigators say metal fatigue caused a hole to rip open in the roof of a Southwest Airlines jet as it cruised at 35,000 feet last year (2009). The National Transportation Safety Board says the 14-inch crack developed in a spot where two sheets of aluminum skin were bonded together on the Boeing 737 jet.• The pilot made an emergency landing in Charleston, W.Va. There were no injuries among the 126 passengers and five crew members. Two months after the scare, Boeing told all airlines with 737s to conduct repeated inspections of the top of the fuselage near the vertical tail fin. The Federal Aviation Administration has since made those inspections mandatory.• Southwest got the plane in 1994 — its much older than the average Southwest jet — and had flown it for 50,500 hours and made 42,500 takeoffs and landings before it sprang a hole in the roof, according to the safety board report. The safety board said it found signs of metal fatigue by magnifying the area in front of the tail fin. In a 3-inch stretch, the crack penetrated completely through the aluminum skin.• FAA records showed that eight cracks had been found and repaired in the fuselage during the planes 14-year checkup.
Fatigue Mechanism• Crack grows incrementally da typ. 1 to 6 = ( ∆K ) m dN ~ ( ∆σ ) a increase in crack length per loading cycle crack origin• Failed rotating shaft -- crack grew even though Kmax < Kc -- crack grows faster as • ∆σ increases Adapted from Fig. 9.28, Callister & • crack gets longer Rethwisch 3e. (Fig. • loading freq. increases. 9.28 is from D.J. Wulpi, Understanding How Components Fail, American Society for Metals, Materials Park, OH, 1985.) 41
Crack growth rate 1. Initially, growth rate is small, but increases with increasing crack length. 2. Growth rate increases with applied stress level for a given crack length (a1).
S-N Curves• A specimen is subjected to stress cycling at a maximum stress amplitude; the number of cycles to failure is determined.• This procedure is repeated on other specimens at progressively decreasing stress amplitudes.• Data are plotted as stress S versus number N of cycles to failure for all the specimen.• Typical S-N behavior: the higher the stress level, the fewer the number of cycles. 43
Fatigue Limit• For some iron and titanium alloys, the S-N curve becomes horizontal at higher number of cycles N.• Essentially it has reached a fatigue limit, and below this stress level the material will not fatigue.• The fatigue limit represents the largest value of fluctuating stress that will not cause failure for an infinite number of cycles. 44
Surface Treatments• During machining operations, small scratches and grooves can be introduced; these can limit the fatigue life.• Improving the surface finish by polishing will enhance fatigue life significantly.• One of the most effective methods of increasing fatigue performance is by imposing residual compressive stresses within a thin outer surface layer. A surface tensile stress will be offset by the compressive stress.• Shot peening (localized plastic deformation) with small (diameters ranging from 0.1 to 1.0 mm), hard particles (shot) are projected at high velocities on to the surface. The resulting deformation induces compressive stresses to a depth of roughly ¼ to ½ of the shot diameter.• The influence of shot peening is compared in the graph. 46
Improving Fatigue Life1. Impose a compressive surface stress (to suppress surface cracks from growing) --Method 1: shot peening --Method 2: carburizing shot C-rich gas put surface into compression 2. Remove stress bad better concentrators. bad better 47
Case Hardening• Case hardening is a technique where both surface hardness and fatigue life are improved for steel alloys.• Both core region and carburized outer case region are seen in image. Knoop microhardness shows case has higher hardness (smaller indent).• A carbon or nitrogen rich outer surface layer (case) is introduced by atomic diffusion from the gaseous phase. The case is typically 1mm deep and is harder than the inner core material. 48
Creep•Materials are often placed in service at elevated temperatures (>0.4 Tm) and exposed to static mechanical stresses.•Examples are turbine rotors in jet engines and steam generators that experience centrifugal stresses and high pressure steam lines.•Creep is time dependent, permanent deformation of the material when subjected to a constant load or stress. 50
Creep• A typical creep test consists of subjecting a specimen to a constant load or stress while maintaining constant temperature.• Upon loading, there is instant elastic deformation. The resulting creep curve consists of 3 regions: primary or transient creep adjusts to the creep level (creep rate may decrease); secondary creep- steady state-constant creep rate, fairly linear region (strain hardening and recovery stage); tertiary creep, there is accelerated Creep strain vs time at constant load and rate of strain until rupture (grain constant elevated temperature. Minimum creep boundary separation, internal rate (steady-state creep rate), is the slope of the crack formation, cavities and linear segment in the secondary region. Rupture voids). lifetime tr is the total time to rupture.
Creep Sample deformation at a constant stress (σ) vs. time σ σ,ε 0 tPrimary Creep: slope (creep rate)decreases with time.Secondary Creep: steady-statei.e., constant slope.Tertiary Creep: slope (creep rate)increases with time, i.e. acceleration of rate. 52
CreepDependence of creep strain rate on stress; stress versus rupturelifetime for a low carbon-nickel alloy at 3 temperatures.
Secondary Creep• Strain rate is constant at a given T, σ -- strain hardening is balanced by recovery stress exponent (material parameter) Qc ε s = K 2σ exp − n activation energy for creep strain rate RT (material parameter) material const. applied stress • Strain rate 200 Stress (MPa) 427°C increases 100 538 °C for higher T, σ 40 20 649 °C 10 10 -2 10 -1 1 Steady state creep rate ε s (%/1000hr) 55
SUMMARY• Engineering materials dont reach theoretical strength.• Flaws produce stress concentrations that cause premature failure.• Sharp corners produce large stress concentrations and premature failure.• Failure type depends on T and stress: - for noncyclic σ and T < 0.4Tm, failure stress decreases with: - increased maximum flaw size, - decreased T, - increased rate of loading. - for cyclic σ: - cycles to fail decreases as ∆σ increases. - for higher T (T > 0.4Tm): - time to fail decreases as σ or T increases. 56